A method to screen and evaluate tissue adhesives for joint repair applications
© Dehne et al.; licensee BioMed Central Ltd. 2012
Received: 13 January 2012
Accepted: 12 September 2012
Published: 17 September 2012
Tissue adhesives are useful means for various medical procedures. Since varying requirements cause that a single adhesive cannot meet all needs, bond strength testing remains one of the key applications used to screen for new products and study the influence of experimental variables. This study was conducted to develop an easy to use method to screen and evaluate tissue adhesives for tissue engineering applications.
Tissue grips were designed to facilitate the reproducible production of substrate tissue and adhesive strength measurements in universal testing machines. Porcine femoral condyles were used to generate osteochondral test tissue cylinders (substrates) of different shapes. Viability of substrates was tested using PI/FDA staining. Self-bonding properties were determined to examine reusability of substrates (n = 3). Serial measurements (n = 5) in different operation modes (OM) were performed to analyze the bonding strength of tissue adhesives in bone (OM-1) and cartilage tissue either in isolation (OM-2) or under specific requirements in joint repair such as filling cartilage defects with clinical applied fibrin/PLGA-cell-transplants (OM-3) or tissues (OM-4). The efficiency of the method was determined on the basis of adhesive properties of fibrin glue for different assembly times (30 s, 60 s). Seven randomly generated collagen formulations were analyzed to examine the potential of method to identify new tissue adhesives.
Viability analysis of test tissue cylinders revealed vital cells (>80%) in cartilage components even 48 h post preparation. Reuse (n = 10) of test substrate did not significantly change adhesive characteristics. Adhesive strength of fibrin varied in different test settings (OM-1: 7.1 kPa, OM-2: 2.6 kPa, OM-3: 32.7 kPa, OM-4: 30.1 kPa) and was increasing with assembly time on average (2.4-fold). The screening of the different collagen formulations revealed a substance with significant higher adhesive strength on cartilage (14.8 kPa) and bone tissue (11.8 kPa) compared to fibrin and also considerable adhesive properties when filling defects with cartilage tissue (23.2 kPa).
The method confirmed adhesive properties of fibrin and demonstrated the dependence of adhesive properties and applied settings. Furthermore the method was suitable to screen for potential adhesives and to identify a promising candidate for cartilage and bone applications. The method can offer simple, replicable and efficient evaluation of adhesive properties in ex vivo specimens and may be a useful supplement to existing methods in clinical relevant settings.
KeywordsTissue adhesive Bonding strength Cartilage Bone Transplant Tissue engineering Joint repair Test method
Tissue adhesives are very useful means in a wide variety of medical procedures such as skin and wound closure , vascular repair [2, 3], bone piece fixation in osteosurgery , and fixation of biomaterials and engineered transplants in cartilage repair .
Several factors influence the success and efficacy of a tissue adhesive like the biocompatibility, biodegradability, cost, availability and the tissue bonding properties . Standardized methods to determine the strength properties of tissue adhesives are made available by standard bodies like the American Society of Testing and Materials (ASTM). These methods provide means for comparison of adhesive strength of tissue adhesives in tension, and in lap-shear or t-peel by tension loading (ASTM test methods: F2255, F2256, F2258). The common and simple structure of these experimental setups covers a broad range of medical bonding problems useful for test substrates from various tissues. Unfortunately, such test conditions often do not sufficiently reflect the biological complexity and the variety of the individual application resulting in a limited predictive power for in vivo testing. Therefore, the development of test methods still remains a key aspect in searching for new tissue adhesives.
In cartilage tissue engineering (TE) the fixation of tissues and transplants in the knee cavity represents a particular challenge, due to the complex mechanical loading condition. Fibrin glue has been widely-used , but it still has drawbacks like the danger to spread diseases  and cause allergenic reactions , and, particularly, a non-sufficient adhesive strength [9, 10]. Hence there is still a high demand for alternative products.
Apart from test methods relating to ASTM, several test methods have been developed to determine adhesive strength in joint tissues. Reindel et al. developed a method to analyze the integrative repair and the adhesive strength at glued cartilage-cartilage interfaces based on thin cartilage stripes . Jürgensen et al. chose for the same purpose osteochondral cylinders . Hunter et al. developed an easy to handle in vitro cartilage repair model to analyze the integration and maturation of transplants . Sierra et al. determined the failure characteristics of multiple-component adhesives . Since these studies mainly focus on bonding properties of newly developed adhesive materials rather than the method itself, the description is often not sufficient to adequately reproduce. The employed equipment is customarily very complex and costly and demands a high level of technical experience and practice.
On the basis of previously published methods and existing standards we developed a method to screen and evaluate tissue adhesives intended for fixating tissues and transplants for joint repair applications. The method employs viable osteochondral tissue from porcine femoral condyles to capture aspects of joint repair applications such as bonding on cartilage and bone tissue, and surgical fixation of tissues and transplants in joint defects. The methodical approach involved steps like the generation of test tissues and the detailed presentation of used equipment and force measurement protocols resulting in an easy to use method for replication. The efficiency of this methodology was demonstrated for the adhesive properties of fibrin glue. A screening of different collagen formulations was performed to demonstrate the potential of the method to identify adhesive candidates for joint repair applications.
Viability of tissue cylinders
Adhesive characteristics of fibrin glue
Varying adhesive strengths were detected in the specific tests. Highest values were obtained in pull-out test systems. Inserted cartilage was fixed by fibrin with an adhesive strength of nearly 30.1 kPa after 30 s assembly time (60 s: 26.5 kPa; -1.1-fold vs. 30 s), fibrin/PGLA-cell-transplant resisted up to 33.7 kPa after 30 s and about 47.2 kPa in average after 60 s (1.4-fold vs. 30 s). After 30 s bonding time, adhesive strength between cartilage surfaces (5.2 kPa) was significantly lower than after 60 s (24.6 kPa; 4.9-fold). In bone tissue lowest adhesive strength of all four applied systems was detected after 30 s (2.6 kPa), which was significantly increased after 60 s (12.1 kPa, 4.7-fold). For all measurements a mixture of adhesion and cohesion failure was observed. In total, adhesive strength of fibrin was increasing with assembly time on average of all operation modes (2.4-fold). Substrate failures have not occurred.
Reusability of substrates was investigated with three sets of cartilage cylinders. During repeated use no significant differences were observed compared to freshly prepared cylinders (p = 0.683, Figure 2b).
Screening for potential tissue adhesives
The test system was used to identify potential tissue adhesives. Since collagen represents a promising material due to its biocompatibility and capability to form a natural bonding to the surrounding tissue, the screening was conducted with seven different formulations and recipes of collagen preparations from porcine skin. The assembly time was kept short (30 s) since preliminary experiments have shown that adhesive strength of collagens did not change with time (<1.1-fold vs. 60 s and 0 s).
In an effort to quantify the adhesive bonding strength of potential medical adhesives, it is important to develop consistent and reproducible test methods for evaluation and comparative purposes. Since adhesives will be used on living tissue, a readily available test system is preferred. Available methods range from highly standardized methods with less consideration of biological aspects to tests on animal models reflecting the full complexity of a surgical problem .
Based on previously published methods [11–13] and on our knowledge with engineered tissues, we designed a test method providing the means to determine adhesiveness in bone and cartilage tissue. The complexity and individuality of differing applications imply that the results of a single test are not suitable for determining adhesive properties without thorough analysis and understanding of the application and adhesive behaviors. Therefore, test conditions have been developed considering surgical procedures such as the fixation of tissue and tissue engineered transplants in cartilage. Thus, not only the strength properties of the tissue adhesive at the bonding layer are considered, but also those of adherends and the behavior at the interface . For bonding problems involving different tissues like bone and cartilage in joint repair, strength measurements with bone and cartilage substrates in isolation facilitate the identification of weaknesses and strength of adhesives, and hence, can contribute to improvements of the bonding material.
To test the bonding properties of tissue adhesives under in vivo-like conditions, vital porcine osteochondral tissue cylinders were used. Viability of the tested tissue was proven 48 h post preparation demonstrating suitability of the fabrication process for the generation of substrate tissue comprising vital cells. Tissues from bovine, ovine and porcine cylinders are preferred due to the easy availability and the fact, that relatively large samples can be harvested from a single source. The application of standard shape tools such as hole punches and tissue holders ensured the fabrication of substrate tissues with reproducible shape. For fibrin testing at cartilage surfaces the possible reusability of the prepared tissue was demonstrated. Although not meeting the high standards of material testing, the use of non-homogeneous (biological) material can be beneficial with regard to interactions between adhesive and tissue.
The efficiency of the method was shown on the basis of adhesive properties of fibrin glue. The varying results in the different test modes demonstrate that adhesives pose specific bonding properties closely related to the geometry of the applied setting. Both pull-out settings, providing a cavity filled with tissue or transplant, seem to be advantageous for fibrin, whereas blunt ends of the tissue on tissue settings are apparently not appropriate to exploit the adhesive potential of fibrin. Although difficult to compare with other studies, Sierra et al. determined similar bonding properties (around 30 kPa) for commercially available fibrin glue  confirming results obtained from pull-out settings. In accordance with the time dependent polymerization of fibrinogen , the test method was able to identify differences in adhesive strength after 30 s and 60 s assembly time. Since the collagen formulations have shown higher adhesiveness in preliminary experiments and to limit the experimental effort, screening experiments were performed only for the short time period.
We observed a mixture of adhesion and cohesion failure when fibrin was tested. Adhesive and cohesive strength determine the bonding effectiveness and can give information about adhesive properties. Ideally, cohesive failure occurs through the insufficient internal strength of the adhesive. Breaks can indicate brittleness and deformations are characteristic for e.g. polymeric elastics. Adhesion failure occurs if mechanical and intermolecular forces at the bonding layer do not resist the load . The type of failure is determined by the lower strength. Combinations of both types can indicate inhomogeneities within the adhesive material or at the bonding layer. The preparation of fibrin can easily lead to inhomogeneities since fibrinogen and thrombin have to be mixed before use by the operator. Furthermore, irregularities at the substrate surface cannot be excluded completely since biological materials naturally vary.
A screening of different collagen formulations was performed to demonstrate the potential of the method to identify a promising candidate. As comparative standard fibrin glue was used, that is widely-used as adhesive in surgery . The results confirm the high bonding strength of fibrin in tests filling defects such as fixing transplants or tissues. Different collagen formulations were generated using different extraction methods (urea, pepsin) and downstream modifications (oxidation, concentration, mixture with hyaluronic acid sodium salt (HA)). A test specimen extracted with pepsin and mixed with HA (sample 3) demonstrated potent adhesive properties in cartilage and bone tissue, but was not suitable for fixing fibrin-based TE transplants in defects. Other specimen extracted with pepsin (sample 5–7) or mixed with HA showed no increase of adhesive strength suggesting the formation of a unique complex between both substances. Furthermore, the varying results in the different test assemblies demonstrate that adhesive properties are closely connected with the requirements, thus, a test method has to be adapted as best to the condition of the intended application.
Generally, the method can be easily changed to torsion and shear measurements applying another force measurements device capable of it. The method was kept simple and all used equipment can easily be obtained from local providers and collaborators. The preparation technique is easily translatable to other models with comparable dimensions of joints like horse, goat and sheep [18–20]. The use of human tissue would be favorable but will be most likely not be in line with ethical considerations. Generally, the data generated from a testing method on biological tissue may vary from that found in vivo, however, testing results can offer valuable information on the potential bonding capacity and the preparation of subsequent in vivo experiments.
The method represents a useful supplement to existing methods to determine adhesive strength in viable tissues in clinical relevant settings, even though not all medical procedures for cartilage or bone surgeries and TE-based interventions are covered. The method was kept simple and replicable since universal equipment was applied and detailed protocols were provided. Different test modes confirmed the dependence of bonding properties and applied settings further justifying individual test methods in addition to standard testing. Finally, the presented method was suitable to screen potential adhesives and to identify a promising candidate for cartilage and bone applications.
The grip for force measurements comprises a cylindrical hole to hold the completed test tissue cylinders. Since tensile and compressive forces do appear during measurements, additional screws ensure adherence to exact position. The other site of the holder was designed to fit into the jig of a force measurement device (Figure 4b).
Preparation of test substrate cylinders
Finally, using raw tissue cylinders as a basis (Figure 5d), it was possible to create plane cartilage and bone tissue cylinders useful to mimic the fixation of these tissues (Figure 5h). Additional cut-outs on raw cylinders with a hole punch (Ø 6 mm Aesculap, Germany, Tuttlingen) were done to generate defined artificial defects (Figure 5f). For adhesive testing, these defects are either filled with cartilage tissue discs obtained from the previous cut-out step or with TE transplants described below (Figure 5g, h). Completed tissue cylinders were maintained until use in chondrocyte culture medium described below.
Test of viability
Test substrate cylinders were examined for tissue viability on 0.5 mm cartilage slices involving propidium iodide/fluorescein diacetate staining (PI/FDA; Sigma-Aldrich, Germany, Taufkirchen) before use in adhesive strength testing (48 hours post preparation). Washing steps were done using PBS (Biochrom). The staining was performed first in FDA solution (3 μg/ml; 15 min, 37°C) and subsequently in PI staining solution (100 μg/ml; 2 min; RT). For microscopy an Olympus CKX41 combined with a reflected fluorescence microscopy system was used (Olympus, Hamburg, Germany). A histomorphometric analysis was performed to determine the percentage of apoptotic cells as a measure for the viability of the tissue. For each PI/FDA image the percentage of red stained areas (pixel) was determined in red-green-blue (RGB) color mode using a programming software (Xcode, Apple Inc.). Since areas containing viable and apoptotic cells appeared as mixed colors, different red tones were discriminated. Areas with high red content (red value × 0.8 > G value + B value) containing exclusively apoptotic cells were weighted as 100% apoptotic. Areas with moderate content (R × 1.0 > R + B) were weighted 50% and with low red content (R × 1.2 > R + B) 25%. Areas with other colors (R × 1.2 < = R + B) were considered as viable. After RGB analysis an image was created visualizing the discriminated areas in different colors (high – red; moderate – orange; low – yellow, other – green).
Preparation of TE transplants
Transplants were generated adhering to protocols already published and clinically applied for matrix associated chondrocyte implantations . Briefly, chondrocytes were enzymatically isolated from porcine femoral condyle cartilage. Cells were sub-cultured in medium (DMEM, Biochrom, Germany Berlin) containing 10% FBS (Biochrom). For storage cells were frozen in 10% DMSO supplemented with 80% serum and 10% medium, and were kept in liquid nitrogen until use. For transplant generation cells were thawed, sub-cultured for two weeks, and resuspended in media containing fibrinogen (33% v/v, Tissucol Duo S, Baxter, Germany, Unterschliessheim). The cell suspension was loaded and incorporated into bioresorbable co-polymer fleeces of poly(lactic-co-glycolic acid) (PLGA, 6 mm diameter, Ethicon, Germany). Addition of thrombin (10% v/v in PBS, Tissucol Duo S) led to polymerization to fibrin resulting in a ready-to-use fibrin/PLGA-cell-transplant.
Determination of the adhesive strength
To determine the adhesive strength, a tensile test was performed. The strength of the bonding was determined using a Zwick Z005 universal testing machine (Zwick GmbH, KG, Germany, Ulm) equipped with 50 N load cell (AST GmhH, Germany, Dresden). The adhesive assembly (test substrate + adhesive) was held at 0.5 N contact load at room temperature for different contact times. Jointing components were merged with a speed of 10 mm/min until contact load was reached. After reaching assembly time, jointing components were pulled apart until rupture at a nominal speed of 5 mm/min while recording load and time. Equal volumes of fibrinogen and thrombin (20 μl each, Baxter) were applied separately on substrate tissue surfaces immediately before starting the measurement sequence. For candidate screening 20 mg material were used. For fibrin and candidate testing at least 5 repetitions were performed with freshly prepared adhesive specimen and substrates. To test the reusability of tissue substrates, three cartilage cylinder sets were used, which were reused up to 10 times.
Modes of operation
The bonding strength was calculated from maximum bonding strength (τmax) subtracted with “no template control” (NTC) bonding strength determined with phosphate buffered saline (PBS, Biochrom, Germany, Berlin). This correction was performed for each series of measurement (Figure 1), since substrate tissues demonstrated low self-adhesive properties.
Preparation of collagen formulations
For screening tests different collagen formulations were randomly generated. Therefore, brine-conserved porcine skin was separated from fat by acetone extraction and concomitant proteins were removed through extraction with a solution containing sodium chloride (6% w/v) and formic acid (1% w/v). Collagen extraction was achieved either through extraction with 6M urea (samples 1, 2 and 4), or through exposure to 5% pepsin (samples 3, 5–7). Except sample 3 pepsin-extracted specimens were further oxidized using sodium periodate (sample 5–7). Samples 6 and 7 were additionally crosslinked with adipic acid dihydrazide. Sample 7 was concentrated by ultrafiltration before crosslinking. Sample 2 and 3 were mixed with same volume of 0.2% hyaluronic acid sodium salt (CPN spol. s r.o., Czech Republic, Dolní Dobrouc).
Significance level of pair wise group comparison has been obtained applying t-test statistics of the SigmaStat 3.5 software package (Statcon, Germany, Witzenhausen). If normality or equal variance test was not passed Wilcoxon rank sum-test was conducted. A p-value lower than 0.05 was considered significant.
TD carried out adhesive strength measurements, assembly of data, data analysis and interpretation, and writing the manuscript. RZ contributed to the collection and interpretation of data, and writing the manuscript. JPK participated in the design and fabrication of custom-made devices and contributed to the development of measurement protocols. AP and RV provided the study material, contributed to the data analysis and interpretation, and participated in writing the manuscript. MS and HS participated in the conception and design of the study. JR conceived of the study, and participated in its design and coordination and helped to draft the manuscript. All authors read and approved the final manuscript.
American society of testing and materials
Dulbecco’s modified Eagle's medium
No template control
Phosphate buffered saline
The authors gratefully thank Barbara Walewska, Larissa Nicolaus and Annette Thiem for excellent technical support, and Kristin Minkwitz for carefully reading of the manuscript and useful comments. This study was supported by grants from the Investitionsbank Berlin and the European Regional Development Fund (grant no: 10140057), and the Berlin-Brandenburg Center for Regenerative Therapies.
- Reece TB, Maxey TS, Kron IL: A prospectus on tissue adhesives. Am J Surg. 2001, 182 (2 Suppl): 40S-44S.View ArticlePubMedGoogle Scholar
- Berthelsen B, Lofgren J, Svendsen P: Embolization of cerebral arteriovenous malformations with bucrylate. Experience in a first series of 29 patients. Acta Radiol. 1990, 31 (1): 13-21.PubMedGoogle Scholar
- Sawamura Y, Asaoka K, Terasaka S, Tada M, Uchida T: Evaluation of application techniques of fibrin sealant to prevent cerebrospinal fluid leakage: a new device for the application of aerosolized fibrin glue. Neurosurgery. 1999, 44 (2): 332-337. 10.1097/00006123-199902000-00048.View ArticlePubMedGoogle Scholar
- Donkerwolcke M, Burny F, Muster D: Tissues and bone adhesives–historical aspects. Biomaterials. 1998, 19 (16): 1461-1466. 10.1016/S0142-9612(98)00059-3.View ArticlePubMedGoogle Scholar
- Spotnitz WD: Fibrin sealant: past, present, and future: a brief review. World J Surg. 2010, 34 (4): 632-634. 10.1007/s00268-009-0252-7.View ArticlePubMedGoogle Scholar
- Spotnitz WD, Burks S: State-of-the-art review: hemostats, sealants, and adhesives II: update as well as how and when to use the components of the surgical toolbox. Clin Appl Thromb Hemost. 2010, 16 (5): 497-514. 10.1177/1076029610363589.View ArticlePubMedGoogle Scholar
- Horowitz B, Busch M: Estimating the pathogen safety of manufactured human plasma products: application to fibrin sealants and to thrombin. Transfusion. 2008, 48 (8): 1739-1753. 10.1111/j.1537-2995.2008.01717.x.View ArticlePubMedGoogle Scholar
- Oswald AM, Joly LM, Gury C, Disdet M, Leduc V, Kanny G: Fatal intraoperative anaphylaxis related to aprotinin after local application of fibrin glue. Anesthesiology. 2003, 99 (3): 762-763.View ArticlePubMedGoogle Scholar
- Baik SH, Kim JH, Cho HH, Park SN, Kim YS, Suh H: Development and analysis of a collagen-based hemostatic adhesive. J Surg Res. 2010, 164 (2): e221-228. 10.1016/j.jss.2010.08.004.View ArticlePubMedGoogle Scholar
- Burke SA, Ritter-Jones M, Lee BP, Messersmith PB: Thermal gelation and tissue adhesion of biomimetic hydrogels. Biomed Mater. 2007, 2 (4): 203-210. 10.1088/1748-6041/2/4/001.View ArticlePubMedPubMed CentralGoogle Scholar
- Reindel ES, Ayroso AM, Chen AC, Chun DM, Schinagl RM, Sah RL: Integrative repair of articular cartilage in vitro: adhesive strength of the interface region. J Orthop Res. 1995, 13 (5): 751-760. 10.1002/jor.1100130515.View ArticlePubMedGoogle Scholar
- Jurgensen K, Aeschlimann D, Cavin V, Genge M, Hunziker EB: A new biological glue for cartilage-cartilage interfaces: tissue transglutaminase. J Bone Joint Surg Am. 1997, 79 (2): 185-193.PubMedGoogle Scholar
- Hunter CJ, Levenston ME: Maturation and integration of tissue-engineered cartilages within an in vitro defect repair model. Tissue Eng. 2004, 10 (5–6): 736-746.View ArticlePubMedGoogle Scholar
- Sierra DH, Eberhardt AW, Lemons JE: Failure characteristics of multiple-component fibrin-based adhesives. J Biomed Mater Res. 2002, 59 (1): 1-11. 10.1002/jbm.1210.View ArticlePubMedGoogle Scholar
- Duda GN, Haisch A, Endres M, Gebert C, Schroeder D, Hoffmann JE, Sittinger M: Mechanical quality of tissue engineered cartilage: results after 6 and 12 weeks in vivo. J Biomed Mater Res. 2000, 53 (6): 673-677. 10.1002/1097-4636(2000)53:6<673::AID-JBM9>3.0.CO;2-V.View ArticlePubMedGoogle Scholar
- Habenicht G: Applied Adhesive Bonding- A Practical Guide for Flawless Results. 2009, Weinheim, WILEY-VCHGoogle Scholar
- Hantgan R, Hermans J, Fowler W, Erickson H: Fibrin formation as a biological assembly process. Biophys J. 1980, 32 (1): 438-440. 10.1016/S0006-3495(80)84973-3.View ArticlePubMedPubMed CentralGoogle Scholar
- Barnewitz D, Endres M, Kruger I, Becker A, Zimmermann J, Wilke I, Ringe J, Sittinger M, Kaps C: Treatment of articular cartilage defects in horses with polymer-based cartilage tissue engineering grafts. Biomaterials. 2006, 27 (14): 2882-2889. 10.1016/j.biomaterials.2006.01.008.View ArticlePubMedGoogle Scholar
- Kangarlu A, Gahunia HK: Magnetic resonance imaging characterization of osteochondral defect repair in a goat model at 8 T. Osteoarthritis and cartilage / OARS, Osteoarthritis Research Society. 2006, 14 (1): 52-62. 10.1016/j.joca.2005.08.006.View ArticlePubMedGoogle Scholar
- Orth P, Goebel L, Wolfram U, Ong MF, Graber S, Kohn D, Cucchiarini M, Ignatius A, Pape D, Madry H: Effect of subchondral drilling on the microarchitecture of subchondral bone: analysis in a large animal model at 6 months. Am J Sports Med. 2012, 40 (4): 828-836. 10.1177/0363546511430376.View ArticlePubMedGoogle Scholar
- Ossendorf C, Kreuz PC, Steinwachs MR, Erggelet C: Autologous chondrocyte implantation for the treatment of large full-thickness cartilage lesions of the knee. Saudi Med J. 2007, 28 (8): 1251-1256.PubMedGoogle Scholar
- The pre-publication history for this paper can be accessed here:http://www.biomedcentral.com/1471-2474/13/175/prepub
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.